TC4 titanium alloy is currently one of the most widely used titanium alloys. It has high strength and good corrosion resistance. However, it is difficult to see seamless titanium tubes made of TC4 in the seamless titanium tube market at home and abroad.
The TC4 titanium material is mainly plate material. The TC4 titanium pipe material on the market is mainly high-strength thick-walled pipe produced by hot extrusion or oblique piercing. This warm rolling process needs to be improved on the traditional roll, that is, on the pipe rolling mill. Install induction heating device, this kind of processing equipment has complicated structure, complicated process and high production cost. The main reason for this current situation is the high strength of TC4 titanium alloy and the difficulty of cold rolling forming. In order to solve the key technology of TC4 seamless tube cold-rolling forming, a series of researches have been carried out jointly by schools and enterprises. For example, the direct cold-rolling forming process is used to produce high-strength titanium alloy pipes, which not only greatly reduces the production cost, but also meets the requirements for high-performance titanium alloy applications.
The billeting method with different deformations is adopted, and the tube blank is rolled into a tube with a total deformation of 70% after two passes and three passes, respectively. 800℃×1h vacuum annealing is carried out between passes. The cooling method is furnace cooling to 500℃ and then air cooling to room temperature to observe the changes in structure and properties. Concluded:
In the case of billeting with small deformation, the wall thickness deviation is small and the surface roughness gradually decreases; for billeting with large deformation, the wall thickness deviation is large, which will affect the wall thickness deviation of the pipes obtained by subsequent passes.
In the case of the same total deformation, the more rolling passes, the greater the elongation and hardness of the pipe, and the higher the strength. Good overall performance.
When rolling with large deformation, the flow of material is strip-shaped, and when rolling with small deformation, the flow of material is bundled. When the heat treatment conditions between passes are the same as the subsequent rolling process, the tube with large deformation is billeted The tissue distortion is more serious.
Small deformation billet has little effect on the anisotropy of the pipe; there are certain fluctuations in the anisotropy of the mechanical properties in multi-pass rolling.
Link to this article：Technology of Cold Rolling TC4 Titanium Alloy Titanium Tube
Reprint Statement: If there are no special instructions, all articles on this site are original. Please indicate the source for reprinting:Alloy Wiki，thanks